- Young's modulus
solid mechanics, Young's modulus (E) is a measure of the stiffnessof an isotropic elastic material. It is also known as the Young modulus, modulus of elasticity, elastic modulus (though Young's modulus is actually one of several elastic moduli such as the bulk modulusand the shear modulus) or tensile modulus. It is defined as the ratio of the uniaxial stress over the uniaxial strain in the range of stress in which Hooke's Lawholds. [GoldBookRef|title=modulus of elasticity (Young's modulus), "E"|file=M03966] This can be experimentally determined from the slopeof a stress-strain curvecreated during tensile tests conducted on a sample of the material.
Young's modulus is named after Thomas Young, the 18th century British scientist. However, the concept was developed in 1727 by
Leonhard Euler, and the first experiments that used the concept of Young's modulus in its current form were performed by the Italian scientist Giordano Riccatiin 1782 — predating Young's work by 25 years. ["The Rational Mechanics of Flexible or Elastic Bodies, 1638-1788": Introduction to Leonhardi Euleri Opera Omnia, vol. X and XI, Seriei Secundae. Orell Fussli.]
Young's modulus is the ratio of stress, which has units of
pressure, to strain, which is dimensionless; therefore Young's modulus itself has units of pressure. A purist might argue that the units are fine if the dimensionless ratio is left in (i.e. lbs/in^2 over in/in). Carrying the full expression can be helpful for canceling units, in dimensional analysis.
SIunit of modulus of elasticity (E, or less commonly Y) is the pascal; the practical units are megapascals (MPa) or gigapascals (GPa or kN/mm²). In United States customary units, it is expressed as pounds (force) per square inch (psi).
The Young's modulus allows the behavior of a bar made of an isotropic elastic material to be calculated under tensile or compressive loads. For instance, it can be used to predict the amount a wire will extend under tension or buckle under compression. Some calculations also require the use of other material properties, such as the
shear modulus, density, or Poisson's ratio.
Linear "versus" non-linear
For many materials, Young's modulus is essentially constant over a range of strains. Such materials are called linear, and are said to obey
Hooke's law. Examples of linear materials include steel, carbon fiber, and glass. Rubberand soils(except at very small strains) are non-linear materials.
Young's modulus is not always the same in all orientations of a material. Most metals and ceramics, along with many other materials, are isotropic: Their mechanical properties "are" the same in all orientations. However, metals and ceramics can be treated with certain impurities, and metals can be mechanically 'worked,' to make their grain structures directional. These materials then become anisotropic, and Young's modulus will change depending on which direction the force is applied from. Anisotropy can be seen in many composites as well. For example,
carbon fiberhas a much higher Young's modulus (is much stiffer) when force is loaded parallel to the fibers (along the grain), and is an example of a material with transverse isotropy. Other such materials include woodand reinforced concrete.Engineers can use this directional phenomenon to their advantage in creating various structures in our environment.
Young's modulus, "E", can be calculated by dividing the tensile stress by the tensile strain:
where:E is the Young's modulus (modulus of elasticity):F is the force applied to the object;:A0 is the original cross-sectional area through which the force is applied;:ΔL is the amount by which the length of the object changes;:L0 is the original length of the object.
Force exerted by stretched or compressed material
The Young's modulus of a material can be used to calculate the force it exerts under a specific strain.
:where F is the force exerted by the material when compressed or stretched by ΔL.
From this formula can be derived
Hooke's law, which describes the stiffness of an ideal spring: : where::
Elastic potential energy
elastic potential energystored is given by the integral of this expression with respect to L:
where Ue is the elastic potential energy.
The elastic potential energy per unit volume is given by::, where is the strain in the material.
This formula can also be expressed as the integral of Hooke's law:
Relation among elastic constants
For homogeneous isotropic materials simple relations exist between elastic constants (Young's modulus "E",
shear modulus"G", bulk modulus"K", and Poisson's ratio"ν") that allow calculating them all as long as two are known::
Young's modulus can vary somewhat due to differences in sample composition and test method. The rate of deformation has the greatest impact on the data collected, especially in polymers. The values here are approximate and only meant for relative comparisons.
[http://www.glassproperties.com/young_modulus/ Glassproperties.com] ] ).]
Impulse excitation technique
List of materials properties
* [http://www.matweb.com Matweb: free database of engineering properties for over 63,000 materials]
Wikimedia Foundation. 2010.